Abstract
Recent years have witnessed tremendous success in the discovery of topological states of matter. Particularly, sophisticated theoretical methods in timereversalinvariant topological phases have been developed, leading to the comprehensive search of crystal database and the prediction of thousands of topological materials. In contrast, the discovery of magnetic topological phases that break time reversal is still limited to several exemplary materials because the coexistence of magnetism and topological electronic band structure is rare in a single compound. To overcome this challenge, we propose an alternative approach to realize the quantum anomalous Hall (QAH) effect, a typical example of magnetic topological phase, via engineering twodimensional (2D) magnetic van der Waals heterojunctions. Instead of a single magnetic topological material, we search for the combinations of two 2D (typically trivial) magnetic insulator compounds with specific band alignment so that they can together form a typeIII brokengap heterojunction with topologically nontrivial band structure. By combining the datadriven materials search, firstprinciples calculations, and the symmetrybased analytical models, we identify eight typeIII brokengap heterojunctions consisting of 2D ferromagnetic insulators in the MXY compound family as a set of candidates for the QAH effect. In particular, we directly calculate the topological invariant (Chern number) and chiral edge states in the MnNF/MnNCl heterojunction with ferromagnetic stacking. This work illustrates how datadriven material science can be combined with symmetrybased physical principles to guide the search for heterojunctionbased quantum materials hosting the QAH effect and other exotic quantum states in general.
Introduction
The quantum anomalous Hall (QAH) effect^{1,2,3}, a zero magnetic field manifestation of the integer quantum Hall effect, originates from the exchange interaction between electron spin and magnetism and exhibits quantized Hall resistance and zero longitudinal resistance. Similar to the quantum Hall effect, the QAH effect harbors dissipationless chiral edge states, thus providing an energyefficient platform for stateoftheart applications in spintronics^{4,5} and quantum computing^{6,7}. Guided by theoretical predictions^{8}, the QAH effect was experimentally demonstrated in the magnetically (Cr or V) doped (Bi, Sb)_{2}Te_{3}^{9,10,11,12}. However, magnetic doping reduces the spinorbit coupling (SOC) strength and thus may drive the system into a trivial phase. It also degrades the sample quality by bringing a large amount of disorder scatterings into the system. Consequently, the critical temperature of the QAH state through the magnetic doping approach is usually below 2 K, an orderofmagnitude lower than the Curie temperature of these compounds. Therefore, it is highly desirable to search for new platforms consisting of stoichiometric materials with intrinsic magnetism to realize high temperature QAH state.
Recent rapid development of twodimensional (2D) layered magnetic insulators has provided an exciting opportunity for the realization of QAH effect in undoped material systems. The QAH effect has been proposed to appear in the heterostructures of topological insulator (TI) and magnetic insulator through the magnetic proximity effect across the interface^{13,14,15,16,17}. Another recent advance is the successful synthesis of a class of intrinsic magnetic TI materials, including MnBi_{2}Te_{4}, MnBi_{2}Se_{4}, and MnSb_{2}Te_{4}^{18,19}, in which Atype antiferromagnetism and topologically nontrivial band structure coexist, leading to the successful observation of the QAH state^{20,21,22}. The QAH effect has also been observed in twisted bilayer graphene^{23,24}.
Results
Discovery workflow for QAH heterojunctions
Despite several recent works^{25,26}, the search for more QAH materials is still challenging because it requires the coexistence of ferromagnetism and topological band structure, which is rare in a single material. In this study, we propose an alternative strategy to realize the QAH effect in 2D magnetic van der Waals (VdW) heterojunctions by combining datadriven discovery of 2D magnetic compounds with a theoretical analysis of topological properties. All the previous works^{13,14,15,16,25,26} on the QAH heterojunctions require at least one intrinsic topological material. In contrast, every QAH VdW heterojunction predicted by our approach can be constructed with two trivial 2D ferromagnetic (FM) insulators. There are three types of heterojunctions, defined by the band alignment between the two constituting materials, as shown in Supplementary Fig. 1. The key idea is to make sure the two FM 2D materials form the socalled typeIII brokengap junction, in which the conductionband minimum (CBM) of one 2D material is lower in energy than the valenceband maximum (VBM) of the other compound at certain highsymmetry momentum, as shown in Fig. 1a. In other words, an inverted (topological) band structure is formed by the heterojunction, rather than one individual material. As this strategy only requires the (valence or conduction) band offset to be larger than the band gap of one of the two 2D materials, it greatly relaxes the stringent conditions for the QAH effect and allows us to develop a systematic approach to identify the candidate compounds for the QAH heterojunctions in 2D magnetic VdW material database.
This approach has been successfully utilized to search for the quantum spin Hall insulators, such as InAs/GaSb quantum wells^{27} and other semiconductor heterojunctions^{28}, but it has not been applied to the search of QAH systems, mainly due to the lack of 2D magnetic materials database. Therefore, a datadriven computational and theoretical search of 2D magnetic materials is called for. Figure 1b summarizes the workflow for our datadriven computational approach, which is carefully designed to incorporate highthroughput calculations at multiple computational levels and symmetrybased physical principles that are critical to quickly identify the most promising candidates hosting the QAH effect. In this initial work, we focus on a family of 2D monolayer MXY compounds (M = metal atoms, X = N, S, Se, Te, Y = F, Cl, Br, I) and predict 46 potential 2D magnetic semiconductors in this family. A database including the information of CBM, VBM, band offset, the orbital nature and the symmetry properties of the conduction and valence bands, and the magnetic anisotropy energies and exchange coupling for each candidate compound is created. Based on this 2D magnetic material database, we identify eight brokengap VdW heterojunctions made from different combination of these compounds to possess inverted band structure.
We next perform a generic symmetry analysis of topological properties for the VdW heterojunctions. This analysis is based on the relationship between topological invariant, the Chern number (CN) that characterizes the QAH effect, and the twofold rotation (C_{2}) eigenvalues^{29,30,31,32,33}. We demonstrate that the CN for the heterojunction must be changed by an odd number when the magnetizations in two magnetic VdW compounds are switched from FM to antiFM (AFM) stacking order. This suggests that the QAH phase must exist for at least one magnetic stacking order.
Finally, we choose MnNF/MnNCl heterojunctions as an example and construct a tightbinding model that captures the main features of the band structure from the realistic material simulations. Based on this tightbinding model, we explicitly compute the CN and the chiral edge states of this heterojunction. Our results show that the QAH phase occurs for the FM stacking order of the magnetization between two materials of the heterojunction and is consistent with our symmetry analysis by computing the C_{2} eigenvalues from firstprinciples calculations.
Prediction of 2D magnetic insulators in MXY compounds
In the past decade, a tremendous amount of computed and experimental material data has been shared in the materials research community through multiple material databases for both bulk^{34,35,36} and 2D inorganic compounds^{37,38,39,40,41}. This offered a vast inorganic materials space that is explorable by datadriven approaches and enabled the datadriven discovery of quantum materials hosting exotic topological phases^{25,26,42,43,44}. Here, our theoretical predictions of 2D heterojunctions that host the QAH effect is motivated by the datadriven discovery of a family of 2D monolayer MXY compounds (M = metal atoms, X = N, S, Se, Te, Y = F, Cl, Br, I) that are predicted to host both FM and nonmetallic ground states. We initiated our material discovery efforts from a material set of around 560 monolayer MXY compounds that are created through elemental substitution based on the existing MXY materials in public 2D materials databases^{37,38,39,40,41}. The datadriven materials discovery process is illustrated in Fig. 1b and more computational details can be found in Supplementary Fig. 2. With FM state as the initial magnetic configuration, through an energy minimization and electron density optimization process, we identified 46 potential magnetic semiconductors (see Supplementary Table 1). 2D FM insulators MnNX and CrCX (X = Cl, Br, I; C = S, Se, Te) have been predicted in previous work^{45,46,47,48}. Our comprehensive study puts this 2D compound family as a great platform for the discovery and design of quantum materials based on 2D magnetic heterojunctions.
Constructed by ten different FM MXY compounds, we propose eight VdW heterojunctions (as listed in Table 1), in which the CBM of one 2D layer (called conduction layer) is below the VBM of the other 2D layer (called valence layer). Thus, all these heterojunctions exhibit the desirable band inversion, as well as smallenough (<6.5%) lattice mismatch, as shown in Table 1. The Curie temperatures (T_{c}) of the these 10 monolayer FM MXY compounds are evaluated by performing MonteCarlo (MC) simulations based on a 2D Heisenberg Hamiltonian model^{49,50}. The interaction types, the values of exchange coupling \(J\) and magnetic anisotropy energy \(A\) are summarized in Fig. 1a and Table 2. Computational details related to magnetic anisotropy energies and exchange coupling interactions are included in the Supplementary Methods 1 and Supplementary Fig. 3. Characterized by high Curie temperature as well as small band gaps, this set of magnetic semiconductor compounds provides a great platform for the design of VdW heterojunctions to realize the QAH effect. The CBM of all the conduction layers and the VBM of all the valence layers are both located at Γ point, facilitating the analysis of brokengap junctions.
Symmetry analysis for the VdW heterojunctions
We next analyze the topological properties of the proposed eight VdW heterojunctions based on the symmetry aspect. The magnetic moments are in the z direction (normal to the 2D planes) for all these magnetic MXY compounds, which reduce their plane groups to p2, generated by \(C_2\) and lattice translations. Putting two 2D materials together to form a heterojunction can preserve the \(p2\) symmetry as long as the magnetic moments of two layers are in the same or opposite directions (named as FM or AFM stacking, respectively). Using C_{2} eigenvalues^{29,30,31,32,33}, we will argue that the two stacking orders result in different CNs once the heterojunctions are in the inverted regime, meaning that at least one way gives QAH heterojunctions.
Owing to \(C_2^2 =  1\), the states at four C_{2}invariant momenta have definite C_{2} eigenvalues \(\pm i\), as exemplified in Fig. 2. The quantity of interest is the total number \(n_ \) of occupied states with C_{2} eigenvalue \( i\) at all \(C_2\)invariant momenta, as
holds for a 2D insulator^{29,30}. To get a clear physical picture, we first neglect the SOC and the interlayer coupling between two layers in the VdW heterojunctions but include the charge transfer that equalizes the chemical potentials of the two layers. Such approximation allows us to treat spin and layer indexes as good quantum numbers (see Fig. 2a, b), and then we can split \(n_ \) into \(n_  = n_{  ,v} + n_{  ,c}\) with \(n_{  ,c}\) and \(n_{  ,v}\) from the conduction and valence layers, respectively. The only difference between the FM and AFM stacking is the relative direction of magnetic moments in the two constituting compounds. Without loss of generality, we reverse the direction of the magnetic moment of the conduction layer when switching the stacking order. Since the magnetization in the valence layer stays fixed, we have \(n_{  ,v}^{FM} = n_{  ,v}^{AFM}\) with the superscripts indicating the stacking order.
To address \(n_{  ,c}\), we further split \(n_{  ,c}\) into \(n_{  ,c} = n_{  ,c,low} + n_{  ,c,high}\), where \(n_{  ,c,low}\) comes from the band that is partially filled (involved in the band inversion) and \(n_{  ,c,high}\) is given by the occupied bands fully below \(E_F\) (see Fig. 2a, b). In the conduction layer, the sign of \(C_2\) eigenvalue of any state is flipped when switching from the FM stacking to the AFM stacking, as the orbital nature is unchanged while the spin direction is reversed. It results in \(n_{  ,c,{\mathrm {high}}}^{\mathrm {AFM}} = 4N_{c,{\mathrm {high}}}  n_{  ,c,{\mathrm {high}}}^{\mathrm {FM}}\), where the prefactor 4 comes from the four \(C_2\)invariant momenta and \(N_{c,{\mathrm {high}}}\) is the number of occupied bands fully below \(E_{\mathrm {F}}\) in the conduction layer. Since only one band from the conduction layer is partially filled and it only contributes to \(n_{  ,c}\) at Γ for the heterojunctions of interest, \(n_{  ,c,low}\) is either 0 or 1, leading to \(n_{  ,c,{\mathrm {low}}}^{\mathrm {AFM}} = 1  n_{  ,c,{\mathrm {low}}^{\mathrm {FM}}}\). In sum, we have \(n_  ^{\mathrm {AFM}} = n_  ^{\mathrm {FM}} + 1 + 4N_{c,{\mathrm {high}}}  2n_{  ,c}^{\mathrm {FM}}\), resulting in
Now we discuss the SOC and the interlayer coupling. The energy scales of these two effects are typically much smaller than the energy scale of the band inversion (i.e., the energy gap at \({\mathrm{{\Gamma}}}\) in this case), which is determined by the hopping and the magnetic exchange coupling. Indeed, as shown by the results from firstprinciple calculations (see details in the Supplementary Fig. 8), the SOC and interlayer coupling do not cancel the existing band inversion or introduce new band inversion in the heterostructures of interest, leaving Eq. (2) unchanged. However, the two effects are still important for our analysis since they open the gap at generic momenta (not \(C_2\)invariant momenta) and enable us to combine Eq. (2) with Eq. (1). (See schematic examples in Fig. 2c, d). As a result, we conclude that the parity of the CN is changed when switching the stacking order of the 2D heterojunction (from FM to AFM or the inverse), and thus at least one of the stacking orders can give nonzero CN.
The remaining question is which stacking order guarantee a nonzero CN for the heterojunctions of interest. Let us assume that the CNs of the two individual materials have the same parity, e.g., both materials have zero CNs, so that the total \(n_ \) of the two materials must be even before forming the heterojunction. Then, the key lies on the \(C_2\) eigenvalues of the two states involved in the band inversion at \({\mathrm{{\Gamma}}}\), i.e., CBM of the conduction layer and VBM of the valence layer in this case. Specifically, if the two states have opposite \(C_2\) eigenvalues for a certain stacking order, \(n_ \) of the heterojunction must differ by 1 from the total \(n_ \) of the two materials before forming the heterojunction (see Fig. 2a). Thus, such stacking order must yield a QAH heterojunction according to Eq. (1). With this principle in mind, we list the \(C_2\) eigenvalues of the VBM and CBM for all FM materials with all magnetic moments fixed in the positive z direction (see Supplementary Table 2). From this list, we can directly read out the \(C_2\) eigenvalues of the two states involved in the band inversion at the \({\mathrm{{\Gamma}}}\) point for any heterojunction with FM stacking, and if they are opposite (same), the heterojunction has nonzero CN for the FM (AFM) stacking.
The QAH effect in MnNF/MnNCl heterojunction
The discussion above based on symmetry eigenvalues is valid for all the eight VdW heterojunctions identified if the magnetic moments are aligned along the z direction, while the topological properties of heterojunctions with inplane magnetization is discussed in the Supplementary Discussion 1 and Supplementary Fig. 4. From Table 2, we notice that the magnetic anisotropy of 5 compounds is outofplane while that of the other five materials is inplane. For the heterojunction consisting of the compounds with inplane easy axis, a small outofplane magnetic field may be required to align the magnetic moments. To conclusively demonstrate the emergence of QAH effect from these 2D magnetic VdW heterojunctions, we focus on a prototype system consisting of two magnetic compounds, MnNF and MnNCl with small band gaps. Both compounds are predicted to host FM ground state, being dynamically and thermally stable (Supplementary Figs. 5–7). The Curie temperatures of these two compounds are evaluated by both HSE06 and PBE + U functionals. We observe that the hybrid function predicts lower transition temperatures than PBE + U for MnNF and MnNCl, owing to the fact that the inclusion of exact exchange in HSE06 functional generates more localized states on Mn atoms and weaker exchange interactions among them. Even in this case, the predicted Curie temperatures for MnNF and MnNCl are 671 K and 592 K, respectively (Fig. 3a), well above room temperature. Both partial density of states and orbitalprojected band structures of MnNF and MnNCl (Fig. 3b) indicate that the conductionband edges of these compounds are mainly d states, while the valenceband edge is derived from N p_{y} states.
Based on the calculated band alignment between the two compounds (as shown in Fig. 3b, c), we expect that a typeIII brokengap heterojunction can be formed with band inversion. As shown in Fig. 3d, we create MnNF/MnNCl VdW heterojunctions with both FM and AFM stacking orders. Atomic structures are relaxed using the hybrid functional (HSE06). The interlayer VdW interaction is evaluated by using the DFTD3 correction method of Grimme et al.^{51}. In the case of FM stacking, without SOC, the crossing between two bands in the same spin channel happens around Γ point, leading to the band inversion of 14.0 meV (Supplementary Fig. 8b), and this crossing is protected by mirror symmetry. The inclusion of SOC can open band gaps at the original crossing points of the two bands located at the \({\mathrm{{\Gamma}}}  X\) line. However, as the SOC is quenched by the crystal environment, this gap is only around 0.5 meV (Fig. 3e). To enhance the gap, a relative shift of the MnNF layer relative to the MnNCl layer by 0.5 Å along the y direction is introduced to break the mirror symmetry (see detailed discussion in the Supplementary Discussion 2) and create a gap around 6.0 meV (Fig. 3f). Furthermore, we observe that the band inversion at Γ point can be controlled by applying a biaxial inplane strain (through deformation potential effects) or an external electric field along z direction (see Supplementary Fig. 9), thus providing effective ways to manipulate both electronic structures and topological properties of VdW heterojunctions. As compared to the strong intralayer magnetic interaction, the interlayer magnetic interaction is very weak. The total energy of the MnNF/MnNCl heterojunction with FM stacking order is only 0.1 meV per primitive cell lower than that with AFM stacking order. This combination of strong intralayer and weak interlayer magnetic couplings indicate that, once a FM (or AFM) stacking of the heterojunction is initialized, the magnetic stacking order will be rather stable, because the flip of one spin would be restrained by the strong intralayer magnetic interaction.
In MnNF and MnNCl, within the p2mm plane group, Mn cations are confined in a quasioctahedral bonding environment associated with a t_{2g}–e_{g} d state splitting. This crystal field splitting (1~2 eV) provides an essential electronic structure scaffold for smallgap FM semiconductors. Orbital analysis confirms that the CBM of MnNF or MnNCl is composed of Mn e_{g} states, whereas the VBM is derived from the interaction between occupied N p states and Mn t_{2g} states. This unique electronic structure feature endows the VBM and CBM of MXY compounds different C_{2} rotational eigenvalues (see Supplementary Tables 1 and 2), which is essential for the emergence of QAH effect in their heterojunctions. From our firstprinciples calculations, the CBM and VBM at the Γ point (zone center) of MnNF and MnNCl have opposite \(C_2\) eigenvalues in the FM configuration, indicating that the heterojunction with FM stacking must have nonzero CN according to the above symmetry analysis. To better understand the result of firstprinciple calculation, we construct effective models around \({\mathrm{{\Gamma}}}\) point near the Fermi energy. Near E_{F}, the conduction and valence bands of both materials are composed of p_{y} and d_{x2−y2} orbitals, respectively (as shown in Fig. 3b, c; x, y, z directions are defined in Fig. 3d). For the FM stacking, the basis can be chosen as (\(\left {d_{x^2  y^2}} \right., \uparrow \rangle\), \(\left {p_y} \right., \uparrow \rangle\)), resulting in the effective model:
Here λ_{1} is given by SOC, all other parameters are dominated by the hopping. More details are provided in the Supplementary Methods 2. According to the band structure from firstprinciples calculations, we may choose \(E_v  E_c\, > \,0\), \(B_{vx}  B_{cx}\, < \,0\), and \(B_{vy}  B_{cy}\, < \,0\). Then, the direct calculation of the CN yields \(CN_{FM}^{eff} =  sgn(A_y\lambda _1)\), which is nonzero. On the other hand, the effective model for AFM stacking has the form:
with bases (\(\left {d_{x^2  y^2}} \right., \uparrow \rangle\), \(\left {p_y} \right., \downarrow \rangle\)) and λ_{0} induced by SOC. The kindependent offdiagonal term leads to CN equals zero. As the occupied bands fully below E_{F} have the same CNs for different stacking orders, the total CNs should differ by one, confirming the above conclusion.
We then construct a tightbinding model for further clarification of the topological properties of the heterostructure. The basis of the model is given by the d_{x}^{2}_{–y}^{2}, d_{xy} and d_{yz} orbitals of the Mn atoms and the p_{y} orbital of the N atoms. The FM of each layer is included by adding the localized magnetic moments on the Mn atoms and the onsite SOC is also included. With reasonable parameter values, the bulk band structures of the FM and AFM stacked heterostructures are shown in Fig. 4a, b, respectively, which qualitatively match those obtained by the firstprinciple calculations (see the Supplementary Methods 2 and Supplementary Fig. 10 for more details). Direct calculations for the FM and AFM stacked heterostructure yield CN = 1 and CN = 0, respectively, coinciding with the chiral edge mode for FM stacking in Fig. 4c and the fully gapped edge for AFM stacking in Fig. 4d. The tightbinding model calculation verifies different topological properties of the FM and AFM stacked heterostructures.
Discussion
In summary, we proposed a new approach to realize the QAH effect in 2D magnetic VdW heterojunctions and conclusively demonstrate the existence of the QAH effect in MnNF/MnNCl heterojunction with FM stacking by combining the firstprinciples calculations and the symmetry analysis. We also proposed other VdW heterojunctions that can host the QAH effect, as listed in Table 1, and the FM stacking always guarantees nonzero CN for them if each individual material is topologically trivial. It is important to note that Mn, Cr, Mo, and W atoms in these compounds that form VdW heterojunctions are all in a d^{3} electronic configuration with t_{2g} states occupied and e_{g} states empty. Given the high Curie temperatures (above room temperature) of many compounds in the MXY family (see Table 2), these VdW heterojunctions provide an ideal platform to explore the possibility of roomtemperature QAH state. The electronic structures and topological properties of VdW heterojunctions can be effectively controlled by strain and electric field (see Supplementary Fig. 9). Moreover, the design principles proposed in this work is not limited to this family of materials and can be extended/applied to a large variety of 2D magnetic systems in multiple plane groups protected by various symmetry operations, which will greatly expand the family of heterojunctionbased QAH systems in the future. Therefore, our work will stimulate experimental synthesis and measurement efforts in this class of heterojunction systems and accelerate the discovery and design of new QAH materials, as well as quantum systems for other magnetic topological phases.
Note added
During the final stage of this work, a related work appeared on arXiv, which performed a systematic search for magnetic topological materials based on magnetic topological quantum chemistry approach^{52}.
Methods
Firstprinciples calculations based on density functional theory
In our calculations, geometric relaxations and total energy calculations were performed using density functional theory within projectoraugmented wave (PAW) potentials^{53,54} as implemented in the VASP code^{55}. A vacuum slab of 20 Å and a planewave basis set with an energy cutoff of 520 eV were used. A 10 × 8 × 1 Γpoint centered kpoint was applied to sample the Brillouin zone. For the initial steps of discovery process, GGA + U was employed to optimize the geometric structures^{56}. The Uvalues are 3.25, 3.7, 3.9, 5.3, 3.32, 6.2, 4.38, and 6.2 eV for V, Cr, Mn, Fe, Co, Ni, Mo, and W, respectively, which are outlined in the work by Wang et al.^{57}. The structures were fully relaxed until energy and force were converged to 10^{−6} eV and 0.01 eV/Å, respectively. The screened hybrid functional of Heyd, Scuseria, and Ernzerhof (HSE06)^{58,59} was used to compute the band structures of MXY monolayers. For the 10 promising FM MXY scaffolding compounds, HSE06 calculations were performed to optimize the geometric structures, and compute the magnetic interactions. To verify the dynamical stability of monolayer MnNF and MnNCl, phonon dispersion analysis was performed by using the density functional perturbation theory method as implemented in the Phonopy code^{60}, interfaced with VASP. In phonon and formation energy calculations, GGA + U along with the PAW potentials were employed, with a convergence criterion of 10^{−8} eV for energy. For the ab initio molecular dynamics (MD) simulations^{61,62}, a canonical (NVT) ensemble was used. Time step for MD simulations is 1 fs.
Data availability
The authors declare that the main data supporting the findings of this study are available within the paper and its Supplementary files. Other relevant data are available from the corresponding author upon reasonable request.
References
Liu, C.X., Zhang, S.C. & Qi, X.L. The quantum anomalous Hall effect: theory and experiment. Annu. Rev. Condens. Matter Phys. 7, 301–321 (2016).
Wang, J., Lian, B. & Zhang, S.C. Quantum anomalous Hall effect in magnetic topological insulators. Phys. Scr. T164, 014003 (2015).
Chang, C.Z. & Li, M. Quantum anomalous Hall effect in timereversalsymmetry breaking topological insulators. J. Phys. Condens. Matter 28, 123002 (2016).
Wu, J., Liu, J. & Liu, X.J. Topological spin texture in a quantum anomalous Hall insulator. Phys. Rev. Lett. 113, 136403 (2014).
Zhang, R.X., Hsu, H.C. & Liu, C.X. Electrically tunable spin polarization of chiral edge modes in a quantum anomalous Hall insulator. Phys. Rev. B 93, 235315 (2016).
Chen, C.Z., Xie, Y.M., Liu, J., Lee, P. A. & Law, K. T. Quasionedimensional quantum anomalous Hall systems as new platforms for scalable topological quantum computation. Phys. Rev. B 97, 104504 (2018).
Zeng, Y., Lei, C., Chaudhary, G. & MacDonald, A. H. Quantum anomalous Hall Majorana platform. Phys. Rev. B 97, 081102 (2018).
Yu, R. et al. Quantized anomalous Hall effect in magnetic topological insulators. Science 329, 61–64 (2010).
Chang, C.Z. et al. Highprecision realization of robust quantum anomalous Hall state in a hard ferromagnetic topological insulator. Nat. Mater. 14, 473–477 (2015).
Chang, C.Z. et al. Experimental observation of the quantum anomalous Hall effect in a magnetic topological insulator. Science 340, 167–170 (2013).
Checkelsky, J. et al. Trajectory of the anomalous Hall effect towards the quantized state in a ferromagnetic topological insulator. Nat. Phys. 10, 731 (2014).
Bestwick, A. J. et al. Precise quantization of the anomalous Hall effect near zero magnetic field. Phys. Rev. Lett. 114, 187201 (2015).
Li, M. et al. Proximitydriven enhanced magnetic order at ferromagneticinsulator–magnetictopologicalinsulator interface. Phys. Rev. Lett. 115, 087201 (2015).
Tang, C. et al. Above 400K robust perpendicular ferromagnetic phase in a topological insulator. Sci. Adv. 3, e1700307 (2017).
Katmis, F. et al. A hightemperature ferromagnetic topological insulating phase by proximity coupling. Nature 533, 513–516 (2016).
Fu, H., Liu, C.X. & Yan, B. Exchange bias and quantum anomalous Hall effect in the MnBi_{2}Te_{4}CrI_{3} heterostructure. Sci. Adv. 6, eaaz0948 (2020).
Zou, R., et al. Intrinsic quantum anomalous Hall phase induced by proximity in germanene/Cr_{2}Ge_{2}Te_{6} van der Waals heterostructure. Phys. Rev. B. 101, 161108 (2020).
Li, J. et al. Intrinsic magnetic topological insulators in van der Waals layered MnBi_{2}Te_{4}family materials. Sci. Adv. 5, eaaw5685 (2019).
Otrokov, M. M. et al. Prediction and observation of an antiferromagnetic topological insulator. Nature 576, 416–422 (2019).
Liu, C., et al. Quantum phase transition from axion insulator to Chern insulator in MnBi_{2}Te_{4}. Preprint at https://ui.adsabs.harvard.edu/abs/2019arXiv190500715L (2019).
Deng, Y. et al. Quantum anomalous Hall effect in intrinsic magnetic topological insulator MnBi_{2}Te_{4}. Science 367, 895–900 (2020).
Ge, J., et al. Highchernnumber and hightemperature quantum Hall effect without Landau levels. Natl. Sci. Rev. 7, 1280 (2020).
Serlin, M. et al. Intrinsic quantized anomalous Hall effect in a moiré heterostructure. Science 367, 900–903 (2020).
Sharpe, A. L. et al. Emergent ferromagnetism near threequarters filling in twisted bilayer graphene. Science 365, 605 (2019).
Choudhary, K., Garrity, K. F., Jiang, J., Pachter, R. & Tavazza, F. Computational search for magnetic and nonmagnetic 2D topological materials using unified spinorbit spillage screening. NPJ Comput. Mater. 6, 1–8 (2020).
Olsen, T. et al. Discovering twodimensional topological insulators from highthroughput computations. Phys. Rev. Mater. 3, 024005 (2019).
Liu, C., Hughes, T. L., Qi, X.L., Wang, K. & Zhang, S.C. Quantum spin Hall effect in inverted TypeII semiconductors. Phys. Rev. Lett. 100, 236601 (2008).
Zhang, H., Xu, Y., Wang, J., Chang, K. & Zhang, S.C. Quantum spin Hall and quantum anomalous Hall states realized in junction quantum wells. Phys. Rev. Lett. 112, 216803 (2014).
Turner, A. M., Zhang, Y., Mong, R. S. K. & Vishwanath, A. Quantized response and topology of magnetic insulators with inversion symmetry. Phys. Rev. B 85, 165120 (2012).
Hughes, T. L., Prodan, E. & Bernevig, B. A. Inversionsymmetric topological insulators. Phys. Rev. B 83, 245132 (2011).
Bradlyn, B. et al. Topological quantum chemistry. Nature 547, 298–305 (2017).
Po, H. C., Vishwanath, A. & Watanabe, H. Symmetrybased indicators of band topology in the 230 space groups. Nat. Commun. 8, 50 (2017).
Kruthoff, J., de Boer, J., van Wezel, J., Kane, C. L. & Slager, R.J. Topological classification of crystalline insulators through band structure combinatorics. Phys. Rev. X 7, 041069 (2017).
Bergerhoff, G., Hundt, R., Sievers, R. & Brown, I. The inorganic crystal structure data base. J. Chem. Inf. Comput. Sci. 23, 66–69 (1983).
Jain, A. et al. Commentary: The Materials Project: a materials genome approach to accelerating materials innovation. APL Mater. 1, 011002 (2013).
Gražulis, S. et al. Crystallography Open Database (COD): an openaccess collection of crystal structures and platform for worldwide collaboration. Nucleic Acids Res. 40, D420–D427 (2011).
Ashton, M., Paul, J., Sinnott, S. B. & Hennig, R. G. Topologyscaling identification of layered solids and stable exfoliated 2D materials. Phys. Rev. Lett. 118, 106101 (2017).
Choudhary, K., Kalish, I., Beams, R. & Tavazza, F. Highthroughput identification and characterization of twodimensional materials using density functional theory. Sci. Rep. 7, 5179 (2017).
Haastrup, S. et al. The computational 2D materials database: highthroughput modeling and discovery of atomically thin crystals. 2D Mater. 5, 042002 (2018).
Mounet, N. et al. Twodimensional materials from highthroughput computational exfoliation of experimentally known compounds. Nat. Nanotechnol. 13, 246 (2018).
Zhou, J. et al. 2DMatPedia, an open computational database of twodimensional materials from topdown and bottomup approaches. Sci. Data 6, 86 (2019).
Zhang, T. et al. Catalogue of topological electronic materials. Nature 566, 475–479 (2019).
Tang, F., Po, H. C., Vishwanath, A. & Wan, X. Comprehensive search for topological materials using symmetry indicators. Nature 566, 486–489 (2019).
Vergniory, M. et al. A complete catalogue of highquality topological materials. Nature 566, 480 (2019).
Guo, Y., Zhang, Y., Yuan, S., Wang, B. & Wang, J. Chromium sulfide halide monolayers: intrinsic ferromagnetic semiconductors with large spin polarization and high carrier mobility. Nanoscale 10, 18036–18042 (2018).
Qi, J., Wang, H. & Qian, X. Electrically tunable, high Curie temperature 2D ferromagnetism in van der Waals layered crystals. Appl. Phys. Lett. 117, 083102 (2020).
Wang, C. et al. A family of hightemperature ferromagnetic monolayers with locked spindichroismmobility anisotropy: MnNX and CrCX (X = Cl, Br, I; C= S, Se, Te). Sci. Bull. 64, 293–300 (2019).
Jiang, Z., Wang, P., Xing, J., Jiang, X. & Zhao, J. Screening and design of novel 2D ferromagnetic materials with high Curie temperature above room temperature. ACS Appl. Mater. Inter. 10, 39032–39039 (2018).
Xiang, H., Lee, C., Koo, H.J., Gong, X. & Whangbo, M.H. Magnetic properties and energymapping analysis. Dalton Trans. 42, 823–853 (2013).
Xiang, H., Kan, E., Wei, S.H., Whangbo, M.H. & Gong, X. Predicting the spinlattice order of frustrated systems from first principles. Phys. Rev. B 84, 224429 (2011).
Grimme, S., Antony, J., Ehrlich, S. & Krieg, H. A consistent and accurate ab initio parametrization of density functional dispersion correction (DFTD) for the 94 elements HPu. J. Chem. Phys. 132, 154104 (2010).
Xu, Y., et al. Highthroughput Calculations of antiferromagnetic topological materials from magnetic topological quantum chemistry. Preprint at https://ui.adsabs.harvard.edu/abs/2020arXiv200300012X (2020).
Blöchl, P. E. Projector augmentedwave method. Phys. Rev. B 50, 17953 (1994).
Kresse, G. & Joubert, D. From ultrasoft pseudopotentials to the projector augmentedwave method. Phys. Rev. B 59, 1758 (1999).
Kresse, G. & Furthmüller, J. Efficiency of abinitio total energy calculations for metals and semiconductors using a planewave basis set. Comput. Mater. Sci. 6, 15–50 (1996).
Dudarev, S. L., Botton, G. A., Savrasov, S. Y., Humphreys, C. J. & Sutton, A. P. Electronenergyloss spectra and the structural stability of nickel oxide: An LSDA+U study. Phys. Rev. B 57, 1505–1509 (1998).
Wang, L., Maxisch, T. & Ceder, G. Oxidation energies of transition metal oxides within the GGA+U framework. Phys. Rev. B 73, 195107 (2006).
Heyd, J., Scuseria, G. E. & Ernzerhof, M. Hybrid functionals based on a screened Coulomb potential. J. Chem. Phys. 124, 219906 (2006).
Heyd, J., Scuseria, G. E. & Ernzerhof, M. Hybrid functionals based on a screened Coulomb potential. J. Chem. Phys. 118, 8207–8215 (2003).
Togo, A. & Tanaka, I. First principles phonon calculations in materials science. Scr. Mater. 108, 1–5 (2015).
Kresse, G. & Hafner, J. Ab initio molecular dynamics for liquid metals. Phys. Rev. B 47, 558–561 (1993).
Kresse, G. & Hafner, J. Ab initio moleculardynamics simulation of the liquidmetal–amorphoussemiconductor transition in germanium. Phys. Rev. B 49, 14251–14269 (1994).
Acknowledgements
We thank Cuizu Chang and Xiaodong Xu for the helpful discussion. J.P. and Q.Y. acknowledge support from the U.S. Department of Energy under Award #DESC0019275 for the design of datadriven discovery pipeline and the firstprinciples computational work. J.Y. and C.X.L. acknowledge the support of DOE grant (DESC0019064) for the analytical model and symmetry analysis, and the Office of Naval Research (Grant number N000141812793), as well as Kaufman New Initiative research grant of the Pittsburgh Foundation. A.J. acknowledges support from U.S. DOE SESC0014388. S.X.D. thanks the International Partnership Program of Chinese Academy of Sciences, Grant number 112111KYSB20160061. It benefitted from the supercomputing resources of the National Energy Research Scientific Computing Center (NERSC), a U.S. Department of Energy Office of Science User Facility operated under Contract number DEAC0205CH11231.
Author information
Authors and Affiliations
Contributions
Q.Y. and C.X.L. conceived and coordinated the research project. J.B.P. and J.Y. contributed equally to this work. J.B.P., Y.F.Z., and Q.Y. implemented the discovery workflow and performed the DFT calculations. J.Y. and C.X.L. performed the symmetry analysis and constructed the effective and tightbinding models. All authors participated in discussing the data and editing the manuscript.
Corresponding authors
Ethics declarations
Competing interests
The authors declare no competing interests.
Additional information
Publisher’s note Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Supplementary information
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Pan, J., Yu, J., Zhang, YF. et al. Quantum anomalous Hall effect in twodimensional magnetic insulator heterojunctions. npj Comput Mater 6, 152 (2020). https://doi.org/10.1038/s4152402000419y
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/s4152402000419y
This article is cited by

Ultrathin lithium aluminate spinel ferrite films with perpendicular magnetic anisotropy and low damping
Nature Communications (2023)

Fabrication and application of arrays related to twodimensional materials
Rare Metals (2022)